- Email: [email protected]

Spatial anisotropy of photoelastic and acoustooptic properties in b-BaB2O4 crystals A.S. Andrushchak a, Y.V. Bobitski b, M.V. Kaidan a, B.V. Tybinka a, A.V. Kityk c,e,*, W. Schranz d a Lviv Politechnic National University, S. Bandery Street 12, 79013 Lviv, Ukraine Institute of Technics, Rzeszow University, ul. Rejtana 16A, 35-959 Rzeszow, Poland Institute for Computer Science, Technical University of Czestochowa, Al. Armii Krajowej 17, 42-200 Czestochowa, Poland d Institut fu¨r Experimentalphysik, Universita¨t Wien, Strudlhofgasse 4, A-1090 Wien, Austria e Economics and Management Department, Polonia University in Czestochowa, 42-200 Czestochowa, Poland b

c

Received 6 May 2004; accepted 10 August 2004

Abstract The paper deals with the spatial anisotropy of photoelastic and acoustooptical properties in b-BaB2O4 (BBO) crystals. Our method is based on the construction and analysis of the indicative surfaces describing the spatial anisotropy of the longitudinal and transverse photoelastic eﬀects. By means of the stereographic projections we have determined the maximum values of photoelastic interaction and the anisotropy power. Having the complete photoelastic tensor we calculated the eﬀective photoelastic constant pef and the eﬃciency of isotropic and anisotropic acoustooptical diﬀractions (the ﬁgure of merit M) for diﬀerent geometries of acoustooptical interactions. The most optimal sample geometries suitable for acoustooptical applications were determined within the computer simulations based on the optimization procedure, namely we have found the sample geometries characterizing by the maximal eﬃciency for the isotropic (M = 6.3 · 1015 s3/kg) and anisotropic (M = 40 · 1015 s3/kg) diﬀractions. Taking into account that BBO is known as a rather strong radiation-steady crystal it may be considered as new eﬃcient acoustooptical material for applications in optical systems with superpower laser irradiation. 2004 Elsevier B.V. All rights reserved. PACS: 42.25.Hz; 42.70.Mp; 78.20.Hp; 78.20.Fm Keywords: b-BaB2O4 crystals; Photoelastic eﬀect; Spatial anisotropy and indicative surfaces, Figure of merit

1. Introduction The beta barium borate (BBO) b-BaB2O4 crystals are known as eﬃcient materials for non-linear optics applications [1,2]. In our previous papers [3–5] we reported the piezooptical properties of these crystals. The results

*

Corresponding author. E-mail addresses: [email protected], (A.V. Kityk).

[email protected]

0925-3467/$ - see front matter 2004 Elsevier B.V. All rights reserved. doi:10.1016/j.optmat.2004.08.075

of these investigations indicate that BBO crystals can be considered also as perspective materials for acoustooptical applications. In this respect further analysis of the photoelastic anisotropy as well as the determination of the ﬁgure of merit in BBO seems to be rather actual. The present paper deals with the spatial anisotropy of photoelastic eﬀect in BBO single crystals. The main purpose of such a study is to determine the geometry of the most eﬀective acoustooptical interaction, i.e., the crystallographic directions for interacting acoustic and optical waves, which are characterized by maximal magnitude of the ﬁgure of merit.

620

A.S. Andrushchak et al. / Optical Materials 27 (2004) 619–624

elastic constants are comparable with corresponding coeﬃcients of fused quartz [9].

2. Calculation of the photoelastic tensor constants The magnitudes of the piezooptical tensor constants pDim (at constant electric displacement D) of BBO crystals have been reported in our recent publications [3–5]. Using these data the piezooptical constants pEim (at constant electric displacement E) can be calculated according to the relation for non-centrosymmetric uniaxial crystals [4,6] pEim pEklgm ¼ pDklgm rkls d sgm =ðeo ðess 1ÞÞ ¼ pDklgm Dklgm ;

ð1Þ

where the second term Dklgm is the secondary electrooptic contribution, rkls and dsgm are the tensor constants corresponding to the linear electrooptic and piezoelectric eﬀects, respectively, e0 = 8.85 · 1012 F/m, ess is the tensor of dielectric constants. For the determination of pEim the following values have been used: r113 = 0.27, r222 = 2.41, r333 = 0.29, r131 = 1.7 and d311 = 1.17; d222 = 2.30; d333 = 3.4; d113 = 9.6 (all values are in 1012 m/V [7]); e11 = e22 = 6.7 and e33 = 8.1 [8]. The photoelastic tensor constants pEin are then expressed as [4,6]: pEin ¼ pEim C mn ¼ pEim S 1 mn ;

ð2Þ

where Cmn is the elastic constant matrix and Smn is the elastic compliance matrix. Our estimations show that the piezoelectric contribution to the elastic compliances of BBO crystals is less than 1% thereby it can be neglected and we will consider that S Dmn ¼ S Emn . For the calculation of the photoelastic constant pEin the magnitudes of elastic compliances Smn are taken from [8], excepting S14 only. The value of this constant is known from our previous experimental measurements [4]. Table 1 lists the calculated values of pEim and pEin constants of BBO crystals as for the temperature of 20 C and the He–Ne laser wavelength k = 632.8 nm. As one can see seen the BBO have rather large magnitudes of photoelastic constants, especially p11 and p12. These crystals have an advantage on such known acoustooptic materials as LiNbO3 or TeO2 and their photoTable 1 The average values of piezooptic constants pDim [3,4], elastic compliance coeﬃcients Smn [6], and calculated values of piezooptic pEim , and photoelasic pEin constants of BBO crystal (as for T = 20 C and k = 632.8 nm) Index im or in

12 2 pD m /N im , Br = 10

pEim , Br

Smn, T Pa1

pEin

11 12 13 31 33 14 41 44

1.7 ± 0.15 1.35 ± 0.08 1.75 ± 0.23 1.6 ± 0.15 3.7 ± 0.37 2.0 ± 0.8 2.03 ± 0.07 26.3 ± 0.9

1.6 1.46 1.73 1.6 3.7 1.54 2.02 26.3

25.63 14.85 9.97 9.97 37.21 22.6 [4] 22.6 [4] 331.3

0.195 0.197 0.059 0.112 0.039 0.005 0.007 0.078

3. The indicative surfaces and their stereographic projections The analysis of spatial anisotropy of the photoelastic properties is based on the indicative surfaces and their stereographic projections. The corresponding method developed in [10] allows to describe both qualitatively and quantitatively the anisotropy of any physical eﬀect in the crystals. We must mention that any ambiguity both in determination of piezo- or photoelastic constants as well as then in the constructing of the indicative surfaces can be removed if to use always the same coordinate system, in particular the one, which was used for the determination of the piezooptic coeﬃcients. In the photoelastic measurements it is important also to choose properly the positive directions of principal coordinate system. This problem has been already discussed in details [11–13]. The equations of the indicative surfaces of the photoelastic eﬀect can be derived in a similar way as for piezooptic eﬀect (see Refs. [3,11]). In the spherical coordinate system (h, u) these equations for BBO crystals get the form: p0ii ðh; uÞ ¼ p11 sin4 h þ ðp13 þ p31 þ 4p44 Þsin2 hcos2 h þ p33 cos4 h þ 2ðp14 þ p41 Þsin3 h cos h sin 3u; ð3Þ 0ðiÞ

pin ðh; uÞ ¼ p12 sin2 h þ p31 cos2 h 2p41 sin h cos h sin 3u; ð4Þ 0ðnÞ

pin ðh; uÞ ¼ p12 sin2 h þ p13 cos2 h 2p14 sin h cos h sin 3u; ð5Þ where p0ii ðh; uÞ is the indicative surface of the longitudi0ðiÞ 0ðnÞ nal photoelastic eﬀect, pin (h, u) and pin (h, u) are the indicative surfaces of the transverse photoelastic eﬀect for light polarization and mechanical deformation, respectively. Fig. 1(a)–(c) shows the indicative surfaces and their stereographic projections (d)–(f) for the longi0 nÞ 0ðiÞ tudinal (p0ii – a; d) and transverse (pin – b, e; pinð – c, f) photoelastic eﬀect in b-BaB2O4 crystals calculated using the Eqs. (3)–(5) and the data (pEin ) presented in the Table 1. More details concerning the method used for a construction of these surfaces is described elsewhere [3,12]. The surfaces were built using the elaborated software by means of meridian and equatorial cross sections with further their projection on the plane. In order to lower shadowing the only upper part of these surfaces are pictured. Complete image of each surface can be represented through an imaginary reproduction relatively to the centre of the coordinate system.

A.S. Andrushchak et al. / Optical Materials 27 (2004) 619–624

621

0ðiÞ

0ðnÞ

Fig. 1. The indicative surfaces (a)–(c) and their stereographic projections (d)–(f) for longitudinal (p0ii – a, d) and transverse (pin – b, e; pin – c, f) photoelastic eﬀect in b-BaB2O4 crystals.

Considering the indicative surfaces as a function of 0ðiÞ 0ðnÞ f(h, u) (i.e. f ðh; uÞ ¼ p0ii ðh; uÞ, pin (h, u) or pin (h, u)) we have calculated the anisotropy power according to the relationship [3] g ¼ ðV sp jV þ V jÞ100%=V sp ;

ð6Þ

3

where Vsp = 4pjfextrj /3 is a sphere volume with radius jfextrj = max(jfminj, jfmaxj), V + and V are the volumes of positive and negative parts of surface, respectively. The anisotropy power deﬁned in such way gives g = 0% when the indicative surface is a sphere whereas if V + = V then the eﬀect has the maximum anisotropy power, i.e. g = 100%. 4. Spatial anisotropy of the photoelastic eﬀect The longitudinal photoelasic eﬀect in BBO crystals (Fig. 1(a)) is characterized by the pronounced anisotropy including the sign inversion. For comparison the

anisotropy of transverse photoelasic eﬀect is less pronounced with the lack of the sign inversion (Fig. 1(b) and (c)). At the same time, the anisotropy power g (see Table 2) calculated according to the Eq. (6) appear to be a bit larger for the indicative surface of the trans0ðnÞ verse eﬀect pin (h, u). In comparison to the piezooptic eﬀect (see paper [3]) the indicative surfaces of the photoelastic eﬀect have essentially smaller (of about two times) value of g, 0ðiÞ 0ðnÞ namely for pin (h, u) and pin (h, u) surfaces. In addition they have much simpler shape and no sign inversion. The latter fact can be explained by the small values of the photoelastic constants p14 and p41 as well as by the same signs of photoelastic constants p12, p13 and p31. Several other features regarding the symmetry follow from the detailed analysis the indicative surfaces in the 0ðiÞ Fig. 1. The surfaces p0ii (h, u) and pin (h, u) clearly do not have a rotation symmetry, what indeed is consistent with the Germans theorem [14]. In fact, these surfaces

Table 2 Extreme values and anisotropy power for the indicative surfaces of the photoelastic eﬀect in BBO crystals (see Fig. 1) Indicative surface p0ii (Fig. 1(a)) 0ðiÞ pin (Fig. 1(b)) 0ðnÞ pin (Fig. 1(c))

Maximal value

Minimal value

Anisotropy power

Magnitude

h

u

Magnitude

h

u

Vsp, (unit)3

jV +V j, (unit)3

g,%

0.039 0.111 0.059

0 5 2

– 30, 150 or 270 30, 150 or 270

0.209 0.198 0.197

67 85 88

30, 150 or 270 90, 210 or 330 90, 210 or 330

0.038 0.032 0.032

0.023 0.021 0.017

39 34 47

622

Table 3 Anisotropy of the acoustooptical properties in BBO crystals (as for T = 20 C and k = 0.6328 lm light wave length) Type of diﬀraction

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20

Isotropic Isotropic Isotropic Isotropic Isotropic Isotropic Isotropic Isotropic* Isotropic** Isotropic Isotropic Isotropic* Isotropic** Anisotropic Anisotropic* Anisotropic** Anisotropic Anisotropic Anisotropic* Anisotropic**

Polarization of optic wave Incidented light il

Diﬀracted light im

h

h

u

[1 0 0] [1 0 0] [1 0 0] [0 1 0] [0 0 1] [0 0 1] [0 1 0] 64 30 56 30 [1 0 0] [1 0 0] 26 30 21 30 [0 1 0] [0 0 1] [0 0 1] [0 1 0] [0 1 0] 4 90 4 210

Acoustic wave Refractive index

u

[1 0 0] [1 0 0] [1 0 0] [0 1 0] [0 0 1] [0 0 1] [0 1 0] 64 30 56 30 [1 0 0] [1 0 0] 26 30 21 30 [0 0 1] [0 1 0] [0 1 0] [0 0 1] [0 0 1] 90 180 90 120

nl = nm = n0 nl = nm = n0 nl = nm = n0 nl = nm = n0 nl = nm = ne nl = nm = ne nl = nm = n0 nl = nm = 1.642 nl = nm = 1.628 nl = nm = n0 nl = nm = n0 nl = nm = 1.571 nl = nm = 1.564 nl = n0; nm = ne nl = ne; nm = n0 nl = ne; nm = n0 nl = n0; nm = ne nl = n0; nm = ne nl = 1.551; nm = n0 nl = 1.551; nm = n0

Propagation a

Polarization f

h

h

u

[1 0 0] [0 1 0] [0 0 1] [1 0 0] [1 0 0] [0 0 1] [0 1 0] 64 30 56 30 [0 1 0] [0 0 1] 26 30 21 30 [1 0 0] 41 90 35 90 [0 0 1] [0 1 0] 4 90 90 120

Mode

Velocity V, 10 m/s

Eﬀective photoelastic constant pef

L QL L L L L QL QL QL QT T QT QT L QL QL T QT QT QT

5.24 5.24 3.73 5.24 5.24 3. 72 5.24 4.82 4.58 0.92 0.93 1.56 1.40 5.24 4.11 3.96 0.93 0.92 0.90 0.88

p11 = 0.195 ~p12 = 0.197 p13 = 0.059 p21 = 0.197 p31 = 0.112 p33 = 0.039 ~p22 = 0.195 ~pef = 0.207 ~pef = 0.204 ~p14 ¼ 0:002 p14 = 0.005 ~pef ¼ 0:094 ~pef ¼ 0:089 p41 = 0.007 ~pef = 0.082 ~pef = 0.079 p44 = 0.078 ~p44 = 0.079 ~pef = 0.079 ~pef = 0.078

a

3

Figure of merit M · 1015, s3/kg

M 0 · 108, m2s/kg

M00 · 1011, ms2/kg

1.48 1.51 0.38 1.51 0.31 0.11 1.48 1.86 1.93 0.015 0.15 6.1 6.3 0.002 0.40 0.44 30 34 36 40

6.8 6.9 0.87 6.9 1.34 0.23 6.8 7.1 6.6 0.002 0.022 2.34 1.94 0.007 1.1 1.1 4.2 4.6 4.7 5.0

1.29 1.32 0.23 1.32 0.26 0.06 1.29 1.47 1.44 0.002 0.024 1.5 1.39 0.001 0.26 0.28 4.5 5.0 5.2 5.7

u

[1 0 0] 89 90 [0 0 1] [1 0 0] [1 0 0] [0 0 1] 89 90 76 30 69 30 1 90 [0 1 0] 121 30.1 114 30.1 [1 0 0] 52 90 44 90 [0 1 0] 1 90 90 180 9.8 30

(*) and (**)-calculated maximum values for eﬀective photoelastic constants pef and ﬁgures of merit M respectively; n0 = 1.550 and ne = 1.667 are the ordinary and extraordinary refractive indices, respectively. a L (QL) and T (QT) are the pure (quasi-) longitudinal and pure (quasi-) transverse acoustic waves, respectively, symbol ‘‘’’ over the notations pin indicates on the eﬀective but not pure photoelastic constant.

A.S. Andrushchak et al. / Optical Materials 27 (2004) 619–624

Sample geometry no.

A.S. Andrushchak et al. / Optical Materials 27 (2004) 619–624

can be described by the point group of symmetry 3 m: a threefold axis and three symmetry planes, which are normal to the (X1, X2) isotropic plane. This corresponds to well-known Neumann principle [15]. At the same time 0ðnÞ the surface pin (h, u) looks like to have the rotation symmetry although the Eq. (5) indeed again predicts the same point symmetry, i.e. 3 m. This can be explained by very small magnitude of photoelastic constant p14 thereby the corresponding weak surface distortions are practically not seen in the Fig. 1(g). As the common feature for all the indicative surfaces of both piezooptic and photoelastic eﬀects is the existence of their circular cross section in the plane normal to the optical axis. It means that at a given deformation, the induced changes of the refractive indices remain constant at any angular position of the light polarization or the direction of the applied uniaxial deformation in the isotropic (X1, X2) plane. This appears to be actual for both longitudinal and transverse photoelastic eﬀects. 0ðnÞ The extreme values of pin (h, u) surface are not shown on the stereographic projection (Fig. 1(g)) since they cannot be determine by means of the Wulﬀ network. How0ðiÞ ever, they as well as the extreme values of pin (h, u) surface can be found numerically by applying the conditions op 0 /oh = 0 and op 0 /ou = 0. Such calculations give the values of about 0.111 and 0.059 together with the following angular coordinates h = 0.5 arctan(2p41/ (p12p31)) 5, u = 30 ± 120 Æ n, where n = 0,1,2,. . . and h = 0.5 arctan(2p14/(p12p13)) 2, u = 30 ± 120 Æ 0 nÞ 0ðiÞ n for the indicative surfaces pin (h, u) and pinð (h, u), respectively (see Table 2). All the rest of extreme values presented in Table 2 were obtained from the numerical analysis or by using the calculated stereographic projections (Fig. 1(d) and (e)) by means of the Wulﬀ network. A zero-isoline, which is presented on the stereographic projection for the longitudinal eﬀect only (see Fig. 1(d)), deﬁnes the set of directions when the photoelastic eﬀect is absent.

623

of acoustic wave. The cases when q = 1 or 2 correspond to a slow or fast transverse acoustic waves, respectively, whereas the case when q = 3 corresponds to the longitudinal acoustic wave. Table 3 presents also the ﬁgures of merit characteristics of BBO crystals calculated as [6,9]: M ¼ p2ef ~n6 =qV 3 , pﬃﬃﬃﬃﬃﬃﬃﬃﬃ M 0 ¼ p2ef ~n7 =qV and M 00 ¼ p2ef ~n7 =qV 2 . Here ~n ¼ nl nm , where nl and nm are the refractive indices of the incident and diﬀracted light, q is the crystal density, V is acoustic wave velocity. In Table 3 the polarizations of optic and acoustic waves are chosen thus that the eﬀective constant of pef coincides with the photoelastic constant pin. The exceptions concern the constants p12 and p22 (see sample geometries No. 2 and No. 7) since the acoustic waves propagating in [0 1 0]-direction are either quasi-longitudinal (QL) or quasi-transverse (QT). For this reason we obtain the diﬀerent values for p14 and ~p14 (sample geometries No. 10 and No. 11) or p44 and ~p44 (sample geometries No. 17 and No. 18) for the acoustic waves propagating along the directions [0 0 1] (with the polarization k[0 1 0]) and [0 1 0] (with the polarization k[0 0 1]). The geometries of the acoustooptical interaction with the maximum magnitudes of the eﬀective elastooptic coeﬃcient pef (marked in the Table 3 as *) and ﬁgure of merit M (marked as **) for diﬀerent types of acoustooptic diﬀraction have been determined within the numerical optimization procedure. According to [9] during the computer simulations we considered only the case when the propagation directions for optic and acoustic waves are orthogonal. By analyzing the data of Table 3 we see that the most eﬃcient acoustooptic interaction in BBO crystals occur for isotropic diﬀraction (sample geometry No. 13, M = 6.3 · 1015 s3/kg) and for anisotropic diﬀraction (sample geometry No. 20, M = 40 · 1015 s3/kg). The latter case is the most attractive speaking about the

5. Figure of merit The magnitude of eﬀective photoelastic constants deﬁnes the eﬃciency of acoustooptical diﬀraction. Table 3 presents the eﬀective photoelastic constants pef calculated according to [6,9] pef ¼ ~il~im ^ p~ a~ fq

ð7Þ

where l, m = 1, 2; q = 1, 2, 3; ~il and ~im are the orts of the polarization directions for incident and diﬀracted light, respectively; ~ a and ~ f q are the orts of the propagation and polarization directions for acoustic wave, respectively; ^ p is the photoelastic tensor. If l = m one deals with the isotropic acoustooptic diﬀraction otherwise (i.e. if l 5 m) the anisotropic type of diﬀraction is considered. According to [9], the symbol q deﬁnes the polarization

Fig. 2. The sample geometry giving the maximum ﬁgure of merit M in b-BaB2O4 crystals (X1, X2, X3 is the crystallophysical reference system; ~ k is the direction of light propagation).

624

A.S. Andrushchak et al. / Optical Materials 27 (2004) 619–624

application aspects of BBO crystals in acoustooptic devices such as modulators and deﬂectors. In details this geometry is shown in the Fig. 2. One should remember that BBO are rather strong radiation-steady crystals [16]. For this reason they may be considered as the perspective acoustooptical materials for application in optical systems with superpower laser irradiation.

6. Conclusion Paper deals with the spatial anisotropy of the photoelastic properties in the b-BaB2O4 crystals. For this reason the indicative surfaces and stereographic projections of longitudinal and transverse photoelastic eﬀects were constructed. We have performed the numerical analysis of the indicative surfaces in order to ﬁnd the geometries with the strongest photoelastic interaction. The anisotropy power is also determined. Having the complete photoelastic tensor we have calculated the eﬀective photoelastic constant pef and the eﬃciency of isotropic and anisotropic diﬀractions (ﬁgure of merit M) for diﬀerent sample geometries of acoustooptical interactions. The most optimal sample geometries were determined within the computer simulations based on the optimization procedure, namely we have found the sample geometries characterizing by maximal eﬃciencies of the isotropic (M = 6.3 · 1015 s3/kg) and anisotropic (M = 40 · 1015 s3/kg) diﬀractions. Taking into account that BBO is known as a rather strong radiation-steady crystals it may be considered as new eﬃcient acoustooptical material for applications in optical systems with superpower laser irradiation.

Acknowledgment This work has been supported by STCU-program (proj. N# 1712 and N# 3222).

References [1] C. Chen, Yi. Wu, K. Li, J. Cryst. Growth 99 (1990) 790. [2] C. Chen, Y. Fan, R.C. Eckord, R.L. Byer, Proceedings of SPIE 68 (1997) 12. [3] A.S. Andrushchak, V.T. Adamiv, O.M. Krupych, I.Yu. Martynyuk-Lototska, Ja.V. Burak, R.O. Vlokh, Ferroelectrics 238 (2000) 299. [4] A.S. Andrushchak, Ya.V. Bobitski, M.V. Kaidan, V.T. Adamiv, Y.V. Burak, B.G. Mytsyk, Opt. Appl. 33 (2003) 345. [5] A.S. Andrushchak, Ya.V. Bobitski, M.V. Kaidan, B.G. Mytsyk, A.V. Kityk, W. Schranz, Opt. Laser Technol., in press. [6] T. Narasimhamurty, Photoelastic and electrooptic properties of crystals, Plenum Press, New-York, London, 1981. [7] L. Bohaty, J. Liebertz, Z. Kristallogr. 192 (1990) 91. [8] D. Eimeri, L. Devis, S. Velsko, E.K. Grahow, A. Zalkin, J. Appl. Phys. 62 (1987) 1968. [9] V.I. Balakshyj, V.N. Parygin, L.E. Chirkov, Fizicheskiye osnovy akustooptiki, Izd. Radio i Svjat, Moscow 1985. [10] Yu.I. Sirotin, M.P. Shaskolskaya, Osnovy kristaloﬁziki, Nauka, Moscow 1975. [11] B.G. Mytsyk, Ya.V. Pryriz, A.S. Andrushchak, Cryst. Res. Technol. 26 (1991) 931. [12] B.G. Mytsyk, A.S. Andrushchak, Crystallogr. Rep. 41 (1996) 1001. [13] B.G. Mytsyk, A.S. Andrushchak, Ukr. Phys. J. 38 (1993) 1015. [14] V.L German, Dokl. Akad. Nauk SSSR 48 (1945) 95. [15] J.F. Nye, Physical Properties of Crystals, Clarendon Press, Oxford, 1992. [16] C. Chen, B. Wu, A. Jiang, G. You, Scientia Sinica Ser. B 28 (1985) 235.

Copyright © 2023 C.COEK.INFO. All rights reserved.